CHAPTER 3 X-RAY DIFFRACTION IN CRYSTAL. X-Ray Diffraction Diffraction of Waves by Crystals X-Ray Diffraction Bragg Equation X-Ray Methods Neutron & Electron Diffraction. Bertha Röntgen’s Hand 8 Nov, 1895. X-RAY.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
CHAPTER 3X-RAY DIFFRACTION IN CRYSTAL
X-Ray
Diffraction
Diffraction of Waves by Crystals
X-Ray Diffraction
Bragg Equation
X-Ray Methods
Neutron & Electron Diffraction
Bertha Röntgen’s
Hand 8 Nov, 1895
Wilhelm Conrad Röntgen
(1845-1923)
=Wavelength , ע = Frequency , c = Velocity of light
x-ray≈ 10-10 ≈1A° E ~ 104 ev
X-RAY TUBE
Evacuated glass bulb
Cathode
Anode
...something
you won't
see very
often
(Visible
Light)
X-ray
An electron in a higher orbital immediately falls to the lower energy level, releasing its extra energy in the form of a photon. It's a big drop, so the photon has a high energy level; it is an X-ray photon.
The free electron collides with the tungsten atom,knocking an electron out of a lower orbital. A higher orbital
electron fills the emptyposition, releasing its excess energy as a photon.
Width b Variable
(500-1500 nm)
Wavelength Constant
(600 nm)
Distance d = Constant
Thus Young’s light interference
experiment proves that light
has wavelike properties.
LIGHT INTERFERENCE
Constructive interference is the result of synchronized light waves that add together to increase the light intensity.
Destructive İnterference . results when two out-of-phase light waves cancel each other out, resulting in darkness.
Single particle
To understand diffraction we also have to consider what happens when a wave interacts with a single particle.The particle scatters the incident beam uniformly in all directions
Solid material
What happens if the beam is incident on solid material? If we consider a crystalline material, the scattered beams may add together in a few directions and reinforce each other to give diffracted beams
A crystal is a periodic structure
( unit cells are repeated regularly)
Solid State Physics deals how the waves are propagated through such periodic structures. In this chapter we study the crystal structure through the diffraction of photons (X-ray), nuetrons and electrons.
The general princibles will be the same for each type of waves.
A crystal behaves as a 3-D diffraction grating for x-rays
W. L. Bragg presented a simple explanation of the diffracted beams from a crystal.
The Bragg derivation is simple but is convincing only since it reproduces the correct result.
Sir William Henry Bragg (1862-1942),
William Lawrence Bragg (1890-1971)
ө
ө
Incident angle
Reflected angle
Wavelength of X-ray
Total Diffracted
Angle
These two x-ray beams travel slightly different distances. The difference in the distances traveled is related to the distance between the adjacent layers.
Connecting the two beams with perpendicular lines shows the difference between the top and the bottom beams.
The line CE is equivalent
to the distance between
the two layers (d)
where, d is the spacing of the planes and n is the order of diffraction.
X-rays are incident at an angle on one of the planes of the set.
There will be constructive interference of the waves scattered from the two successive lattice points A and B in the plane if the distances AC and DB are equal.
If the scattered wave makes the same angle to the plane as the incident wave
The diffracted wave looks as if it has been reflected from the plane
We consider the scattering from lattice points rather than atoms because it is the basis of atoms associated with each lattice point that is the true repeat unit of the crystal; The lattice point is analoque of the line on optical diffraction grating and the basis representsthe structure of the line.
Coherent scattering from a single plane is not sufficient to obtain a diffraction maximum. It is also necessary that successive planes should scatter in phase
Third-order reflection from (111) plane
(333) reflection
which makes n-th order diffraction off (hkl) planes of spacing ‘d’ look like first-order diffraction off planes of spacing d/n.
The GENERAL PRINCIBLES of X-RAY STRUCTURE ANALYSIS to DEDUCE the STRUCTURE of NaCl and KCl
Bragg used an ordinary spectrometer and measured the intensity of specular reflection from a cleaved face of a crystal
found six values of for which a sharp peak in intensity occurred, corresponding to three characteristics wavelengths (K,L and M x-rays) in first and second order (n=1 and n=2 in Bragg law)
Details of structure were than deduced from the differences between the diffraction patterns for NaCl and KCl.
Since Bragg's Law applies to all sets of crystal planes, the lattice can be deduced from the diffraction pattern,makinguse of general expressions for the spacing of theplanesin terms of their Miller indices. For cubic structures
Note that the smaller the spacing the higher the angle of diffraction, i.e. the spacing of peaks in the diffraction pattern is inversely proportional to the spacing of the planes in the lattice. The diffraction pattern will reflect the symmetry properties of the lattice.
A simple example is the difference between the series of (n00) reflections for a simple cubic and a body centred cubic lattice. For the simple cubic lattice, all values of n will give Bragg peaks.
However, for the body centred cubic lattice the (100) planes are interleaved by an equivalent set at the halfway position. At the angle where Bragg's Law would give the (100) reflection the interleaved planes will give a reflection exactly out of phase with that from the primary planes, which will exactly cancel the signal. There is no signal from (n00) planes with odd values of n. This kind of argument leads to rules for identifying the lattice symmetry from "missing" reflections, which are often quite simple.
There are many types of X-ray camera to sort out reflections from different crystal planes. We will study only three types of X-ray photograph that are widely used for the simple structures.
Single
Crystal
Film
X-Ray
Single
Crystal
Film
X-Ray
Lattice constant of the crystal can be determined by means of this method; for a given wavelength if the angle at which a reflection occurs is known, can be determined.
Film
The reflected beams are located on the surface of imaginary cones. By recording the diffraction patterns (both angles and intensities) for various crystal orientations,one can determine the shape and size of unit cell as well as arrangement of atoms inside the cell.
If a powdered specimen is used, instead of a single crystal, then there is no need to rotate the specimen, because there will always be some crystals at an orientation for which diffraction is permitted. Here a monochromatic X-ray beam is incident on a powdered or polycrystalline sample.
This method is useful for samples that are difficult to obtain in single crystal form.
The powder method is used to determine the value of the lattice parameters accurately. Lattice parameters are the magnitudes of the unit vectors a, b and c which define the unit cell for the crystal.
For every set of crystal planes, by chance, one or morecrystals will be in the correct orientation to give the correct Bragg angle to satisfy Bragg's equation. Every crystal plane is thus capable of diffraction. Each diffraction line is made up of a large number of small spots, each from a separate crystal. Each spot is so small as to give the appearance of a continuous line.
A very small amount of powdered material is sealed into a fine capillary tube made from glass that does not diffract x-rays.
The specimen is placed in the Debye Scherrer camera and is accurately aligned to be in the centre of the camera. X-rays enter the camera through a collimator.
The powder diffracts the x-rays in accordance with Braggs law to produce cones of diffracted beams. These cones intersect a strip of photographic film located in the cylindrical camera to produce a characteristic set of arcs on the film.
When the film is removed from the camera, flattened and processed, it shows the diffraction lines and the holes for the incident and transmitted beams.
XRD is a nondestructive technique. Some of the uses of x-ray diffraction are;
Advantages;
Disadvantage;
Different radiation source of neutron or electron can also be used in diffraction experiments.
The physical basis for the diffraction of electron and neutron beams is the same as that for the diffraction of X rays, the only difference being in the mechanism of scattering.
E = p2/2m p = h/λ
E=Energy λ=Wavelength
p=Momentum
mn=Mass of neutron = 1,67.10-27kg
Neutron diffraction has several advantages over its x-ray counterpart;
Electron diffraction has also been used in the analysis of crystal structure. The electron, like the neutron, possesses wave properties;
Electrons are charged particles and interact strongly with all atoms. So electrons with an energy of a few eV would be completely absorbed by the specimen. In order that an electron beam can penetrate into a specimen , it necessitas a beam of very high energy (50 keV to 1MeV) as well as the specimen must be thin (100-1000 nm)
If low electron energies are used, the penetration depth will be very small (only about 50 A°), and the beam will be reflected from the surface.Consequently, electron diffraction is a useful technique for surface structure studies.
Electrons are scattered strongly in air, so diffraction experiment must be carried out in a high vacuum. This brings complication and it is expensive as well.